||This article may require cleanup to meet Wikipedia's quality standards. The specific problem is: There exist more applications than mentioned yet (January 2017) (Learn how and when to remove this template message)|
An epitaxial wafer (also called epi wafer, epi-wafer, or epiwafer) is a wafer of semiconducting material made by epitaxial growth (epitaxy) for use in photonics, microelectronics or photovoltaics. The epi layer may be the same material as the substrate, typically monocrystaline silicon, or it may be a more exotic material with specific desirable qualities.
Silicon epi wafers were first developed around 1966, and achieved commercial acceptance by the early 1980s. Methods for growing the epitaxial layer on monocrystalline silicon or other wafers include: various types of chemical vapor deposition (CVD) classified as Atmospheric pressure CVD (APCVD) or metal organic chemical vapor deposition (MOCVD), as well as molecular beam epitaxy (MBE). Two "kerfless" methods (without abrasive sawing) for separating the epitaxial layer from the substrate are called "implant-cleave" and "stress liftoff". A method applicable when the epi-layer and substrate are the same material employs ion implantation to deposit a thin layer of crystal impurity atoms and resulting mechanical stress at the precise depth of the intended epi layer thickness. The induced localized stress provide a controlled path for crack propagation in the following cleavage step. In the dry stress lift-off process applicable when the epi-layer and substrate are suitably different materials, a controlled crack is driven by a temperature change at the epi/wafer interface purely by the thermal stresses due to the mismatch in thermal expansion between the epi layer and substrate, without the necessity for any external mechanical force or tool to aid crack propagation. It was reported that this process yields single atomic plane cleavage, reducing the need for post lift-off polishing, and allowing multiple reuses of the substrate up to 10 times.
The epitaxial layers may consist of compounds with particular desirable features such as gallium nitride (GaN), gallium arsenide (GaAs), or some combination of the elements gallium, indium, aluminum, nitrogen, phosphorus or arsenic.
Photovoltaic research and development
Solar cells, or photovoltaic cells (PV) for producing electric power from sunlight can be grown as thick epi wafers on a monocrystalline silicon "seed" wafer by chemical vapor deposition (CVD), and then detached as self-supporting wafers of some standard thickness (e.g., 250 µm) that can be manipulated by hand, and directly substituted for wafer cells cut from monocrystalline silicon ingots. Solar cells made with this technique can have efficiencies approaching those of wafer-cut cells, but at appreciably lower cost if the CVD can be done at atmospheric pressure in a high-throughput inline process. In September 2015, the Fraunhofer Institute for Solar Energy Systems (Fraunhofer ISE) announced the achievement of an efficiency above 20% for such cells. The work on optimizing the production chain was done in collaboration with NexWafe GmbH, a company spun off from Fraunhofer ISE to commercialize production. The surface of epitaxial wafers may be textured to enhance light absorption. In April 2016, the company Crystal Solar of Santa Clara, California, in collaboration with the European research institute IMEC announced that they achieved a 22.5% cell efficiency of an epitaxial silicon cell with an nPERT (n-type passivated emitter, rear totally-diffused) structure grown on 6-inch (150 mm) wafers. In September 2015 Hanwha Q Cells presented an achieved conversion efficiency of 21.4% (independently confirmed) for screen-printed solar cells made with Crystal Solar epitaxial wafers.
In 2016, a new approach was described for producing hybrid photovoltaic wafers combining the high efficiency of III-V multi-junction solar cells with the economies and wealth of experience associated with silicon. The technical complications involved in growing the III-V material on silicon at the required high temperatures, a subject of study for some 30 years, are avoided by epitaxial growth of silicon on GaAs at low temperature by Plasma-enhanced chemical vapor deposition (PECVD)
- Swinger, Patricia. Building on the Past, Ready for the Future: A Fiftieth Anniversary Celebration of MEMC Electronic Materials, Inc.. The Donning Company, 2009.
- Swinger, pp. 20, 21, 40, 47.
- Claeys, Cor L. (2006). High Purity Silicon 9, Issue 4. The Electrochemical Society. p. 162. ISBN 9781566775045.
- Hua, Y. N. Identification of Silicon Crystalline Defects on Epi-Wafer in Wafer Fabrication. Chartered Semiconductor Mfg. Ltd., 2001.
- Szweda, R. Diode Laser Materials & Devices – A Worldwide Market & Technology Overview to 2005. Elsevier, 2001. p. x.
- Swinger, pp. 20–22.
- III-V Integrated Circuit Fabrication Technology: Fabrication, Integration and Applications. CRC Press. 2016. pp. 97–136. ISBN 9789814669313.
- US 9336989, Henley, Francois J., "Method of cleaving a thin sapphire layer from a bulk material by implanting a plurality of particles and performing a controlled cleaving process", published 10 May 2016
- Farah, John; Nicholson, John; Thirunavukkarasu, Sekar; Wasmer, Kilian (2014). "Dry-epitaxial lift-off for high efficiency solar cells". 2014 IEEE 40th Photovoltaic Specialist Conference: 1796–1801. doi:10.1109/PVSC.2014.6925271. ISBN 978-1-4799-4398-2.
- III-V Integrated Circuit Fabrication Technology: Fabrication, Integration and Applications. CRC Press. 2016. ISBN 9789814669313.
- Rachow, Thomas; Heinz, Friedemann; Steinhauser, Bernd; Janz, Stefan; Reber, Stefan (2014). "Epitaxial n- and p-type Emitters for High Efficiency Solar Cell Concepts". Journal of Energy and Power Engineering. 8. David Publishing. pp. 1371–1377. Retrieved October 15, 2015.
- Janz, Stefan; Reber, Stefan (14 September 2015). "20% Efficient Solar Cell on EpiWafer". Fraunhofer ISE. Retrieved October 15, 2015.
- Drießen, Marion; Amiri, Diana; Milenkovic, Nena; Steinhauser, Bernd; Lindekugel, Stefan; Benick, Jan; Reber, Stefan; Janz, Stefan (2016). "Solar Cells with 20% Efficiency and Lifetime Evaluation of Epitaxial Wafers". Energy Procedia. 92: 785–790. doi:10.1016/j.egypro.2016.07.069. ISSN 1876-6102.
- Gaucher, Alexandre; Cattoni, Andrea; Dupuis, Christophe; Chen, Wanghua; Cariou, Romain; Foldyna, Martin; Lalouat, Loı̈c; Drouard, Emmanuel; Seassal, Christian; Roca i Cabarrocas, Pere; Collin, Stéphane (2016). "Ultrathin Epitaxial Silicon Solar Cells with Inverted Nanopyramid Arrays for Efficient Light Trapping". Nano Letters. 16 (9): 5358. Bibcode:2016NanoL..16.5358G. doi:10.1021/acs.nanolett.6b01240. PMID 27525513.
- Chen, Wanghua; Cariou, Romain; Foldyna, Martin; Depauw, Valerie; Trompoukis, Christos; Drouard, Emmanuel; Lalouat, Loic; Harouri, Abdelmounaim; Liu, Jia; Fave, Alain; Orobtchouk, Régis; Mandorlo, Fabien; Seassal, Christian; Massiot, Inès; Dmitriev, Alexandre; Lee, Ki-Dong; Cabarrocas, Pere Roca i (2016). "Nanophotonics-based low-temperature PECVD epitaxial crystalline silicon solar cells". Journal of Physics D: Applied Physics. 49 (12): 125603. doi:10.1088/0022-3727/49/12/125603. ISSN 0022-3727.
- Prophet, Graham (18 April 2016). "Cheaper solar cells through kerfless wafers". EE Times (Europe). European Business Press SA. Retrieved 3 January 2017.
- V. Mertens, S. Bordihn, A. Mohr, K. Petter, J. W. Müller, D. J. W. Jeong, R. Hao, T. S. Ravi, “21.4% Efficient Fully Screen Printed n-Type Solar Cell on Epitaxially Grown Silicon Wafers With Built-In Boron Rear Side Emitter“, in Proc. 31st EUPVSEC, Hamburg, Germany 2015, pp. 1000–1002.
- Kobayashi, Eiji; Watabe, Yoshimi; Hao, Ruiying; Ravi, T. S. (2015). "High efficiency heterojunction solar cells on n-type kerfless mono crystalline silicon wafers by epitaxial growth". Applied Physics Letters. 106 (22): 223504. doi:10.1063/1.4922196. ISSN 0003-6951.
- Cariou, Romain; Chen, Wanghua; Maurice, Jean-Luc; Yu, Jingwen; Patriarche, Gilles; Mauguin, Olivia; Largeau, Ludovic; Decobert, Jean; Roca i Cabarrocas, Pere (2016). "Low temperature plasma enhanced CVD epitaxial growth of silicon on GaAs: a new paradigm for III-V/Si integration". Scientific Reports. 6: 25674. doi:10.1038/srep25674. ISSN 2045-2322. PMC . PMID 27166163.